REVIEW

Mie resonance-based dielectric metamaterials

Mie resonance-based dielectric metamaterials Increasing attention on metamaterials has been paid due to their exciting physical behaviors and potential applications. While most of such artificial material structures developed so far are based on metallic resonant structures, Mie resonances of dielectric particles open a simpler and more versatile route for construction of isotropic metamaterials with higher operating frequencies. Here, we review the recent progresses of Mie resonance-based metamaterials by providing a description of the underlying mechanisms to realize negative permeability, negative permittivity and double negative media. We address some potential novel applications. Qian Zhao1,2, Ji Zhou1,*, Fuli Zhang3, Didier Lippens3 1 State Key Lab of New Ceramics and Fine Processing, Department of Materials Science and Engineering, Tsinghua University, Beijing, PRC 2 State Key Lab of Tribology, Department of Precision Instruments and Mechanology, Tsinghua University, Beijing, PRC 3 Institut d’Electronique de Micro-électronique et de Nanotechnologie, UMR CNRS 8520, University of Lille 1, Villeneuve d’Ascq Cedex, France *E-mail: [email protected]

Metamaterials are artificial electromagnetic media structured on

opening the effective parameter space, so that new functionalities

a scale much shorter than their operating wavelength. Under this

in the light scattering can be envisaged.

condition they can be considered as homogeneous media whose

values of the effective permittivity and permeability was also

than periodic effects as it is the case for photonic crystal or more

recognized as one of the major goals of this research area. Great

generally electromagnetic band gap material. Their basic cells

progress in electromagnetic metamaterials has been achieved for

are generally constituted of resonant inclusions which yield a π

these unique physical properties and novel potential applications,

phaseshift in the material response above the resonant frequency.

such as negative refraction2, 3, perfect lens4, 5 and cloaking6-8 have

As a consequence, their effective permittivity and permeability

been shown. They have been experimentally demonstrated in a

can be negative either in separate or overlapping frequency

frequency range from the radio frequencies9 to millimeter waves10,

bands, a unique and distinct property that is not observed in

infrared wavelengths11-13, and visible optics14. Up to date, most

naturally occurring

materials1

. For the latter condition they can

be considered as double negative or negative index media hence

60

Also recently, the achievement of near-zero or less than unity

electromagnetic properties rely mainly on the basic cell rather

DECEMBER 2009 | VOLUME 12 | NUMBER 12

of metamaterials are constructed with the use of sub-wavelength resonant metallic elements. For instance, the first left-handed

ISSN:1369 7021 © Elsevier Ltd 2009

Mie resonance-based dielectric metamaterials

(a)

(b)

(c)

(d)

REVIEW

Fig. 1 Electric and magnetic field distribution in a dielectric cube with the magnetic field polarized along the z axis and electric field polarized along the y axis. (a) Electric field in the plane z=0 near the first Mie resonance. (b) Magnetic field in the plane y=0 near the first Mie resonance. (c) Electric field in the plane z=0 near the second Mie resonance. (d) Magnetic field in the plane y=0 near the second Mie resonance. (Reprinted with permission from37. © 2008 American Physical Society.)

metamaterials (LHMs) with simultaneously negative permittivity and

Mie resonance of particles

permeability have been fabricated by means of metallic split ring

From the viewpoint of scattering theory, all scattering objects can

resonators (SRRs) and wires15, 16, for tailoring the magnetic and electric

be represented by effective electric and/or magnetic polarizability

responses, respectively. Other metallic elements, such as Ω-shaped

densities. Light scattering by small (relative to the incident light

structures17, 18, U-shaped structures19, staplelike structures20, paired

wavelength) spherical particles is a fundamental topic in classical

rods21, dendritic22 and fishnet structures23, are also successfully used

electrodynamics35, and is based upon the exact Mie solution of the

to fabricate LHMs.

diffraction problem36. The scattered field of a single isolated dielectric

Usually, the metallic constitutive elements have conductive loss and

sphere with radius r0 and relative refractive index n can be decomposed

anisotropic electromagnetic responses. Several authors have suggested

into a multipole series with the 2m-pole term of the scattered electric

methods24-26 to construct isotropic metamaterials by combining

field proportional to

metallic SRRs and wires. However it is difficult to fabricate the bulk arrays of complex geometry with submicron or nanoscale sizes in

am =

order to generate a negative permeability effect at infrared and optical frequencies27. Recently, another route based on the interaction between

dielectric inclusions provide a novel mechanism for the creation of magnetic or electric resonance based on displacement currents, and

(1)

whereas the 2m-pole term of the scattered magnetic field is proportional to

electromagnetic waves and dielectric particles28, 29 was proposed to achieve the electric or magnetic resonances. The Mie resonances of

nψ m (nx)ψ m' ( x) − ψ m ( x)ψ m' (nx) nψ m (nx)ξ m' ( x) − ξ m ( x)ψ m' (nx)

bm =

ψ m (nx)ψ m' ( x) − nψ m ( x)ψ m' (nx) ψ m (nx)ξ m' ( x) − nξ m ( x)ψ m' (nx)

(2)

where x=k0r0, k0 is the free-space wavenumber, and ψm(x) and

offer a simpler and more versatile route for the fabrication of isotropic

ξm(x) are the Riccati-Bessel functions. The primes indicate derivation

metamaterials operating at higher frequencies. The progress on metallic

with respect to the arguments. The scattering coefficient am and

elements-based metamaterials has been reviewed in many articles30-32

bm are related to the electric and magnetic responses of the sphere,

and books33, 34. In this review, we focus on the scattering mechanisms

respectively. From the Mie theory we can calculate the electric and

based on Mie resonance in dielectric particles and describe the recent

magnetic dipole coefficients, a1 and b1, respectively. From effective

progress in these metamaterials including ferroelectric and polaritonic

medium theory, we know that these are the multipole terms which

particles and their tunable behaviors.

contribute most significantly to the effective permittivity and

DECEMBER 2009 | VOLUME 12 | NUMBER 12

61

REVIEW

Mie resonance-based dielectric metamaterials

μ eff

⎛ ⎜ 3v f = μ 1 ⎜1 + ⎜ F (θ ) + 2bm −vf ⎜ F (θ ) − bm ⎝

⎞ ⎟ ⎟ ⎟ ⎟ ⎠

(4)

where

F (θ ) =

2(sin θ − θ cosθ ) (θ 2 − 1) sin θ + θ cosθ

be = ε 1 ε 2 , bm = μ1 μ 2

(5)

(6)

The volume fraction of the spherical particles,

4 r v f = π ( 0 ) 3 , θ = k 0 r0 ε 2 μ 2 , r0 and p are the particle radius and 3 p Fig. 2 Calculated effective permittivity εeff and permeability μeff of the magnetodielectric sphere arrays composite. (Reprinted with permission from29. © 2003 IEEE.)

the lattice constant, respectively. Eq 5 shows that F(θ) is a resonant

permeability of the particle composite. Since the magnetic response of

values of F(θ) with a magnitude on the order of unity as given by

a nonmagnetic particle is usually weak, it is important to strengthen

Eqs. (3) and (4).

function and becomes negative above resonance in some range of θ, resulting in the negative permittivity or permeability for negative

In Lewin’s model, the constitutive parameters were formulated

the electromagnetic resonant behavior. For the lowest resonant frequencies of a1 and b1, the sphere exhibits electric and magnetic

only considering the spheres resonating either in the first or second

dipoles. This conclusion can be assessed from the electromagnetic

resonant modes of the Mie series. This is because the higher order Mie

intensity distributions in a high dielectric ceramic cube for a plane

resonances often occur at frequencies beyond the long wavelength

incident wave propagating along the x axis37 (Fig. 1). It can be seen

limit, and thus the Clausius-Mossotti equation does not apply. Then,

that the electric or magnetic fields are mainly localized in the cubes.

Jylha et al.39 improved those formulations by taking into account the

The azimuthal component of the displacement current inside each

electric polarizabilities of spheres operating in the magnetic resonant

cube is greatly enhanced at the first Mie resonance (Fig. 1a) resulting

modes. Independent of Lewin’s model, O’Brien and Pendry28 showed that a

in a large magnetic field along the z axis (Fig. 1b) which corresponds to the TE011 Mie resonance mode. At the second Mie resonance, the

negative effective permeability can be obtained in a two-dimensional

y component of the displacement current inside the cubes increases

array of ferroelectric rods with the magnetic field polarized along the

dramatically (Fig. 1c) and hence with a large magnetic field along

axes of the rods. Although the underlying physics is the same, the

the azimuth (Fig. 1d), which corresponds to the TM011 Mie resonance

authors used another method40 (transfer matrix method) to find the

mode.

effective media values with similar conclusion. The aforementioned

These electric and magnetic dipole resonances act as artificial

theoretical results show that a high permittivity microstructured

‘atoms’ which form the basis of new optical materials. In a material

medium can exhibit isotropic negative values of the effective

made up of a collection of such resonant particles, their combined

permeability and permittivity.

scattering response can act like a material with almost arbitrary values of effective permittivity and permeability. This idea can be verified by using the model proposed in 1947 by

Lewin38

who considered the

electromagnetic scattering properties of a composite material which

With the rapid development of LHMs, Lewin’s model was reconsidered

was constituted of an array of lossless magnetodielectric spheres (ε2

and introduced into the realm of metamaterials to realize single and

and μ2) embedded in another background matrix (ε1 and μ1). The

double negative media. Based on Lewin’s model, Holloway et al.29

effective permittivity εeff and permeability μeff expressions based on

numerically demonstrated the feasibility of achieving simultaneously negative εeff and μeff in the magnetodielectric sphere arrays for

Mie theory are as follows38.

ε eff

62

Mie resonance as a new route for metamaterials

⎛ ⎜ 3v f = ε 1 ⎜1 + ⎜ F (θ ) + 2be −vf ⎜ F (θ ) − be ⎝

⎞ ⎟ ⎟ ⎟ ⎟ ⎠

DECEMBER 2009 | VOLUME 12 | NUMBER 12

wavelengths where the electric and magnetic resonances are excited in the spheres. Eqs. (3) and (4) show that εeff and μeff depend on the (3)

permeability and permittivity of the dielectric inclusions and host medium, as well as the volume fraction of spheres of radius r0. Fig. 2 shows εeff and μeff calculated for υf = 0.5, ε1 = μ1 = 1, ε2 = 40, and

Mie resonance-based dielectric metamaterials

REVIEW

μ2 = 200 as a function of k0r0. There are two regions where both εeff and μeff become negative with the bandwidths becoming narrower by

(a)

decreasing the volume fraction υf. From a practical point of view, many kinds of materials and shapes of particles have been proposed in the literature to fabricate negative or less than unity permeability and permittivity dielectric metamaterials operating in different frequency regions. The designing ideas are summarized in the following.

Magnetic response The realization of abnormal permeability is a tricky issue for various metamaterials, because the magnetic response of materials is usually

(b)

weak, especially at infrared or visible frequencies. Lewin’s model shows that two methods based on Mie resonance can be used to achieve a negative effective permeability effect. The first one is to use magnetodielectric inclusions with large values of permeability and permittivity. The second method is to use nonmagnetic dielectric particles with extremely large permittivity values. In the former case, two terms be and bm in Eqs. (3) and (4) contribute to the negative permeability, while only be plays an important role for the latter. The possibility to use magnetodielectric particles has been numerically demonstrated29. However a magnetodielectric particle with

(c)

simultaneously large values of permittivity and permeability seems physically unattainable even in the microwave. Eq. (4) indicates that nonmagnetic spheres with very high permittivity values can also be employed to induce negative permeability and permittivity effects at the different Mie resonance frequencies. Polaritonic materials, such as ionic solids and polar semiconductors, or ferroelectric materials can provide the large permittivity. For ferroelectric materials, their extreme high permittivity values can be preserved at least up to millimeter wavelengths41. At infrared frequencies however a roll-off of the dielectric constant is observed so that they cannot be used in this frequency range. In contrast, the lattice resonance in polaritonic crystals can be exploited to tailor the permittivity resonance at infrared and optical frequencies. As a consequence, the polaritonic resonance of crystals could be potentially used in the infrared spectral region. The relative permittivity is42

⎛ ⎞ ω2 −ω2 ⎟⎟ , ε r (ω ) = ε (∞)⎜⎜1 + 2 L 2 T ω − ω − i ω γ T ⎝ ⎠

Fig. 3 A three-dimensional dielectric composite with isotropic negative permeability. (a) Photograph of BST cubes arrayed in Teflon substrate. (b) Transmission for the dielectric cube array only (dashed line), wire array only (dotted line), and the combination of BST cubes and wires (solid line). Inset of Fig. 3(b) shows the measured and calculated transmission phase. (c) Retrieved refractive index and permeability (inset). (Reprinted with permission from37. © 2008 American Physical Society.)

experimentally demonstrated in the microwave region37. The dielectric (7)

where ε(∞) is the high-frequency limit of the permittivity, ωT and

cube side length l was 1.0 mm for a lattice constant of 2.5 mm. And the first TE and TM resonance modes, i.e., magnetic and electric resonances were determined by transmission measurements at 6.12

ωL are the transverse and longitudinal optical phonon frequencies, and

and 8.28 GHz respectively. Using smaller cubes (l =0.75 mm) with

γ is the damping coefficient. Therefore, large values of εr(ω) can be

a magnetic resonance near 8.5 GHz, in conjunction with an electric

achieved near the transverse phonon frequency.

response from metallic wires, researchers fabricated double negative

A three-dimensional dielectric composite consisting of an array

media. The results of transmission measurements are displayed in

of dielectric cubes [Ba0.5Sr0.5TiO3 (BST)] with a relative permittivity

Fig. 3b and the retrieved electromagnetic parameters (Fig. 3c) further

of 1600 in a Teflon substrate was fabricated (Fig. 3a) to demonstrate

verified the negative permeability near the first Mie resonance.

the feasibility of this full dielectric metamaterial route. On this basis, isotropic negative values of the effective permeability were

A rectangular dielectric block43 and piezoelectric disks44 were also experimentally verified to design very low-loss magnetic metamaterials.

DECEMBER 2009 | VOLUME 12 | NUMBER 12

63

REVIEW

Mie resonance-based dielectric metamaterials

(a)

(b)

Fig. 4 Schematic of metamaterials based on Mie resonance. (a) A two-dimensional lattice structure for one dielectric-resonator in the cutoff microwave waveguide. (Reprinted with permission from45. © 2007 IEEE.) (b) Terahertz metamaterial consisting of polycrystalline TiO2 cubes-arrays on the Al2O3 substrate. (Reprinted with permission from48. © 2008 Metamaterials.)

Also a two-dimensional square lattice of dielectric disk inserted between two metallic parallel-plate waveguide (Fig. 4a) was also used

(a)

to demonstrate negative refraction, where the macroscopic behavior of dielectric disk provides negative effective permeability and the waveguide plays a role in a TE cut-off waveguide leading to negative effective permittivity45. A dielectric block [(Zr,Sn)TiO4 ceramics, dielectric constant 36.7] with a thin metallic rod screwed inside was proposed to fabricate gradient metamaterial lenses and numerically demonstrated to deflect and focus the incident plane waves46. Dielectric-resonator-based composite right/left-handed transmission lines used to the design of leaky wave antenna can alleviate the significantly large conducting loss and increase the radiation efficiency47. Terahertz metamaterials based

(b)

on the Mie resonance of polycrystalline TiO2 cubes-arrays on the Al2O3 substrate (Fig. 4b) were also experimentally demonstrated by Shibuya et al.48, in which the negative permeability and permittivity occur around 0.28 and 0.38 THz, respectively. A three-dimensional collection of polaritonic spheres was proposed to obtain isotropic negative effective permeability near the first Mie resonance at infrared frequencies49. The calculated effective parameters (LiTaO3 crystal) reported in this reference are shown in Fig. 5 and the isotropy of electromagnetic properties was also verified by a comparison with a full multiple scattering approach. Semiconductor nanoparticles, such as CuCl with a Z3 exciton line at 386.93 nm, Cu2O

Fig. 5 The calculated effective relative permeability (a) and permittivity (b) of a collection of LiTaO3 spheres. (Reprinted with permission from49. © 2005 American Physical Society.)

with a 2P exciton50, and GaP51 were also suggested to realize negative permeability within and below the optical region. Metal nanoclusters

64

Similar to spherical or cubic dielectric elements, the cylindrical

possessing large permittivity at visible frequency can also be used to

particles can also generate the Mie electromagnetic resonances.

obtain magnetic Mie resonance52, 53.

The most important issue is to determine the resonant modes. For

DECEMBER 2009 | VOLUME 12 | NUMBER 12

Mie resonance-based dielectric metamaterials

REVIEW

Pendry et al.59 suggested a metallic wire array structure to realize a

a TE polarization (E field perpendicular to the rod axis), the lowest Mie resonance mode (TE0) corresponds to the magnetic response,

plasma-like state. With such a configuration, the negative permittivity

resulting in negative permeability values. A two-dimensional array of

frequency range can be tuned by the lattice constant and the wire

ferroelectric rods28, 54 and polaritonic rods55 were proposed to obtain

diameter in the low frequency spectral region even at microwave

negative effective permeability56, which can be considered as the

frequencies. Additionally, negative dielectric permittivity can also be

TE0 mode. For TM polarization (E field parallel to the rod axis), the

obtained in more ordinary dielectric media with bound charges, within

lowest two Mie resonances modes, TM0 and TM1, correspond to the

a frequency band above a resonance frequency, where the resonant

electric and magnetic responses, and consequently lead to negative

Lorentz permittivity occurs58.

permittivity and permeability, respectively. The electromagnetic field

Another method is to use the electric resonant mode of the Mie

distribution displayed for the TM1 mode (Fig. 6) can further clarify the

resonance of dielectric particles. For the dielectric sphere or cube, it can

magnetic resonance mechanism57. The electric field is distributed along

be equivalent to a dipole at the second resonant mode as exemplified

the ± z directions with opposite signs along the propagation direction

by the field mapping shown in Fig. 1. For a dielectric column particle,

(Fig. 6b), accounting for a strong circular displacement current (Fig. 6d).

it can be equivalent to an electric dipole at the first resonance mode

Such displacement current results in a large magnetic field along the y

(TM0) and can result in negative permittivity.

axis (Fig. 6c), which corresponds to the TM1 mode.

Negative refraction Electric response

The mechanisms of electric and magnetic resonances in dielectric

An electric response can be accomplished with simpler metallic

particles (spheres, cubes or rods) have been analyzed above. Negative

structures, such as uncoupled rods or strips. The first method to

refraction can be fulfilled by combing the two resonances together.

obtain negative permittivity is the bulk metals at optical frequencies,

However, the first electric resonance (TM mode) is at a higher

where conduction electrons can be assumed to be reasonably free and

frequency than the fundamental magnetic resonance (TE mode) for

plasma-like behavior is responsible for a negative dielectric permittivity

the identical sphere. Due to the different resonance frequencies of TE

at frequencies less than the plasma

frequency58.

Usually, the plasma

and TM modes in the different-sized particles, we can consider the

frequencies of metals are at ultraviolet frequencies and dissipation is

conditions when the first lowest resonance of TM011 mode related

small. As the frequency is much lower than the plasma frequency, the

to a bigger sphere coincides with the TE011 resonance in a smaller

imaginary part of the complex permittivity increases dramatically while

sphere. Recently, Vendik et al.60, 61 numerically studied an artificial

very large negative values of the real part are obtained.

double negative media whose basic unit cell is composed by two

(a)

(b)

(c)

(d)

Fig. 6 Electric and magnetic field distributions in a dielectric rod at the second resonant mode (TM1 mode). (a) Unit cell configuration. (b) Electric field distribution. (c) Magnetic field distribution. (d) Equivalent current ring. (Reprinted with permission from57. © 2007 American Physical Society.)

DECEMBER 2009 | VOLUME 12 | NUMBER 12

65

REVIEW

Mie resonance-based dielectric metamaterials

dielectric spheres of different sizes. The larger sphere was used for the negative permittivity while the small one allows achieving a negative

(a)

permeability in the same microwave frequency band. At the same time, two sets of spheres, having the same size but different materials, were also developed to realize negative refraction62. More recently, a threedimensional isotropic negative-index composite at infrared or visible frequencies was reported51, 63-66. The proposed homogeneous isotropic structures consist of dielectric spheres (gallium phosphide) embedded randomly in a negative permittivity host medium (Cesium)51, or two interpenetrating lattices of spheres63-66. One lattice ensures a negative permeability using a polaritonic material (LiTaO3, SiC, CuCl) and the other lattice creates a negative permittivity effect by using a plasmonic

(b)

material (n-type Ge, Au, MgB2). Negative refraction index effect exists not only in the situation of a regular lattice arrangement but also for randomly distributed nanoparticles when the losses are ignored. However, the numerical results also demonstrated that the negative refraction could not be achieved owing to the large imaginary part of the wave vector corresponding to evanescent rather than propagating waves when the losses of the constitutive materials were taken into account. Another method to fabricate isotropic LHMs based on Mie resonance is using only one kind of micron-scale non-magnetic coated

spheres67-69.

(c)

The underlying physical mechanisms correspond

to a negative effective permeability effect due to polaritonic sphere core while a negative effective permittivity effect results from an electric-dipole resonance of sphere coating on its outer surface whose dispersion follows a Drude model. For an isolated sphere, an electric dipole resonance can be driven when its material permittivity is -2. Since this permittivity value is negative, the electric field is evanescent within the sphere so that such electric dipole resonance is a surface resonance in contrast to the volume effect of the magnetic resonance. Therefore, the coating can be designed to have a negative permittivity. Note that the magnetic resonance of the core is hardly affected, as long as the permittivity of the coating remains small

Fig. 7 The effective (a) permeability, (b) permittivity, and (c) index of a collection coated spheres. The cores are made of LiTaO3 with radius 4 μm, and the coatings are a Drude material with radius 0.7 μm. (Reprinted with permission from70. © 2006 American Physical Society.)

in comparison to the large permittivity of the core. The spheres with a core of a polaritonic crystal LiTaO3 and the coated thin layer

resonance modes of SiC particles at mid-IR under various polarization

of a Drude model semiconductor (or a polaritonic material) were

conditions. Also they proposed to obtain a negative refractive index by

used to demonstrate isotropic negative refraction70. The calculated

combining the two resonances of TM0 and TM1 modes (Fig. 8).

effective electromagnetic parameters are shown in Fig. 7. Such three-

rods in s-polarized light was presented recently. The authors claimed

can be used to realize subwavelength imaging71 and electromagnetic

that large wavelength-to-period ratios do not necessarily result in an

transparency72, 73.

isotropic metamaterial. They also suggested that silicon rod arrays

Besides dielectric spheres array, the electric and magnetic Mie

66

A theory on the electric and magnetic dipole activities of dielectric

dimensional LHMs consisting of metal-coated semiconductor spheres

could exhibit a true metamaterial left handed dispersion branch in

resonances in dielectric rods can also be used to achieve negative

the visible to mid-IR despite the moderate value of the refractive

permittivity and permeability values. Under TM illumination, a

index (n~3.5)75. Such a conclusion is interesting by considering Mie

resonant permittivity due to the TM0 mode excitation and a resonant

resonance in moderate permittivity materials in optics. It has however

permeability due to the TM1 mode excitation can be used to realize

to be checked by experiments in order to discriminate negative

negative permittivity and permeability, respectively. Schuller et al.74

refraction effects resulting from the conventional band folding in

experimentally and numerically observed and identified the Mie

the diffraction regime76 from pure left handed branch effects in the

DECEMBER 2009 | VOLUME 12 | NUMBER 12

Mie resonance-based dielectric metamaterials

REVIEW

(a)

(b)

Fig. 10 Schematic of a cylindrical non-magnetic cloak for TE polarization at mid-infrared. (Reprinted with permission from78. © 2008 Optical Society of America.)

waves and realize invisibility cloak6. Effective permeability can be less than unity around the magnetic resonance and such metamaterials have been suggested to construct invisibility cloak7, 8. An all-dielectric Fig. 8 (a) Calculated effective permeability for a normal incidence TE illuminated array of infinitely long SiC rods. (b) Calculated permittivity (permeability) due to excitation of the zeroth (first) order TM mode. (Reprinted with permission from74. © 2007 American Physical Society.)

cloak (Fig. 9) consisting of radially positioned micrometer-sized ferroelectric cylinders was suggested to perform cloaking at 0.58 THz, which exhibits a strong magnetic resonance based on Mie theory77. At last, Silicon Carbide (SiC) rod, a polaritonic material with phonon resonance bands centered around 12.5 μm, was also suggested to built

(a)

(b)

transparency cloak (Fig. 10) at mid-infrared with the TE resonance mode78. To sum up, an all-dielectric configuration provides an attractive route for designing cloaking devices at microwave, terahertz and infrared frequencies.

Tunable Mie resonance-based metamaterials (c)

(d)

As seen in the previous sections, resonance effects in the electric and magnetic responses appear as a necessary condition for fabricating left-handed metamaterials. Such resonances are strongly dependent on the geometrical dimensions and on the dielectric properties of the constitutive elements. Usually negative values can only be achieved over a narrow frequency range near the resonances, especially for the

Fig. 9 (a) Schematic of a terahertz all-dielectric cloak. Steady-state Ez pattern calculated at 0.58 THz for a copper rod without (b) and with cloak (c). (d) Magnified view of the field pattern of (c). (Reprinted with permission from77. © 2008 Optical Society of America.)

magnetic resonance. From the application point of view, and for a deeper understanding of the intrinsic properties of negative media, it is desirable to implement structures with tunable and reconfigurable resonant properties79. Some tunable metamaterials based on the

long wavelength regime. A verification of negative refraction in a TM

metallic structures have been proposed by modifying the locally

illuminated array of large permittivity ceramic rods was experimentally

dielectric or permeability environment. For example, a control of the

verified at microwave frequencies, corresponding to the combination of

electric and magnetic responses of SRRs and related configurations was

TM0 and TM1 modes57.

experimentally demonstrated through photoexcitation of free carriers in a GaAs substrate80, electrically or magnetically controlled liquid

All-dielectric cloaks

crystals81, 82, along with electrorehological fluids83, 84, ferroelectric85,

Conformal transformation of electromagnetic domains has been

ferromagnetic materials86-89 and other methods90. All these examples

proposed as an exciting approach to control the flow of propagating

correspond however to anisotropic tunable metamaterials whereas

DECEMBER 2009 | VOLUME 12 | NUMBER 12

67

REVIEW

Mie resonance-based dielectric metamaterials

the sample temperature. For a proof of this principle, a simple cubic lattice of ceramic cubes of 0.45 mm side length (BST doped with 5wt% MgO) were arrayed in a Teflon substrate with a lattice constant of 1.25 mm. The microwave scattering parameters were measured under various temperature conditions (Fig. 11a, b). The magnetic resonance corresponding to the first Mie resonance in the dielectric cubes can be continuously and reversibly adjusted from 13.65 GHz to 19.28 GHz (a)

with a temperature changing from -15˚C to 35˚C. The frequency dependence of the effective permeability, displayed in Fig. 11c, shows that negative permeability values can be achieved in a frequency band of about 6 GHz by a temperature variation of 50˚C. It is believed that this temperature controlled metamaterial could be used for the design of adaptive three-dimensional metamaterials and invisibility cloaks which exhibit basically a very narrow fractional bandwidth of the order of 1%93. Another method used to adjust the negative refraction of Mie resonance is to alter the dielectric property of the background medium. Khoo et al.94 proposed nanospheres dispersed liquid crystals to realize

(b)

tunable negative–zero–positive index of refraction in the optical and terahertz regimes.

Outlook As an alternative method for the design of electromagnetic metamaterials, the dielectric particles show several advantages, notably in terms of isotropic parameters, and the fabrication techniques targeting at higher frequencies of operation. Although several experimental demonstrations have allowed the verification of the first principles at microwave and terahertz frequencies, it appears that the research on this area is at a very primary stage with numerous (c)

theoretical and numerical studies. Further experimental works are expected at mid-term in order to demonstrate the possibility of fabricating isotropic negative index material notably in the infrared and visible frequency ranges. Towards this goal the challenging issues

Fig. 11 The actively modulated isotropic negative permeability dielectric composite. (a) Dependence of the first magnetic resonance on the temperature. (b) Dependence of transmission phases on the temperature. (c) Calculated effective permeability under different temperature. (Reprinted with permission from91. © 2008 American Institute of Physics.)

are the preservation of large dielectric constant and low loss in these frequency ranges, which appear as the necessary condition to operate in the long wavelength regime. The introduction of active materials may alleviate or even overcome the problem of intrinsic losses95. At last the inexpensive chemical methods, such as colloidal crystallization,

isotropic properties can be more suitable for potential applications

may be suitable for the synthesis of nanoparticles96, 97. Although much

notably for all angle negative refraction.

work is needed before practical implementations are possible, dielectric

The first dynamic tuning of isotropic metamaterial relying on Mie resonance has been demonstrated recently by altering the dielectric property of the basic

cell91.

As expected from the Mie resonance

metamaterials are a promising candidate for real-world application of the many exciting opportunities provided by electromagnetic metamaterials.

theory, at the first resonance the dielectric sphere is equivalent to a magnetic dipole with a resonance frequency ω ≈ πc /(r0 ε 2 )

Acknowledgments

within the long-wavelength limit. Usually, the permittivity of the

This work is supported by the National Science Foundation of China under Grant Nos. 50425204, 50621201, 50632030, 60608016 and 10774087, and by the State Key Lab of Tribology under Grant No. SKLT 08B12. D.L. would like also to thank the Delegation Générale pour l’Armement for its support in the framework of the contract 06.34.021.

high κ ceramic inclusions varies as a function not only of the local field, but also of temperature92. Therefore, a variation of the effective permeability of the composite material can be realized by changing

68

DECEMBER 2009 | VOLUME 12 | NUMBER 12

Mie resonance-based dielectric metamaterials

REVIEW

Reference 1. Pendry, J. B., Nature Mater. (2006) 5, 763.

49. Wheeler, M. S., et al., Phys. Rev. B (2005) 72, 193103.

2. Shelby, R. A., et al., Science (2001) 292, 77.

50. Yannopapas, V., and Vitanov, N. V., Phys. Rev. B (2006) 74, 193304.

3. Houck, A. A., et al., Phys. Rev. Lett. (2003) 90, 137401.

51. Seo, B. J., et al., Appl. Phys. Lett. (2006) 88, 161122.

4. Pendry, J. B., Phys. Rev. Lett. (2000) 85, 3966.

52. Wu, Q., and Park, W., Appl. Phys. Lett. (2008) 92, 153114.

5. Fang, N., et al., Science (2005) 308, 534.

53. Rockstuhl, C., et al., Phys. Rev. Lett. (2007) 99, 017401.

6. Pendry, J. B., et al., Science (2006) 312, 1780.

54. Felbacq, D., and Bouchitte, G., New J. Phys. (2005) 7, 159.

7. Schurig, D., et al., Science (2006) 314, 977.

55. Huang, K. C., et al., Appl. Phys. Lett. (2004) 85, 543.

8. Cai, W., et al., Nat. Photonics (2007) 1, 224.

56. Felbacq, D., and Bouchitte, G., Phys. Rev. Lett. (2005) 94,183902.

9. Wiltshire, M. C. K., et al., Science (2001) 291, 849.

57. Peng, L., et al., Phys. Rev. Lett. (2007) 98, 157403.

10. Zhang, F. L., et al., Appl. Phys. Lett. (2008) 93, 083104.

58. Ramakrishna, S. A., Rep. Prog. Phys. (2005) 68, 449.

11. Dolling, G., et al., Science (2006) 312, 892.

59. Pendry, J. B., Phys. Rev. Lett. (1996) 76, 4773.

12. Linden, S., et al., Science (2004) 306, 1351.

60. Vendik, O. G., and Gashinova, M. S., in Proceedings of the 34th European Microwave Conference, Amsterdam (IEEE Press, Piscataway, NJ, 2004), Vol. 3, pp. 1209-1212.

13. Liu, H., et al., Adv. Mater. (2008) 20, 2050. 14. Dolling, G., et al., Opt. Lett. (2007) 32, 53. 15. Pendry, J. B., et al., IEEE Trans. Microw. Theory Tech. (1999) 47, 2075. 16. Smith, D. R., et al., Phys. Rev. Lett. (2000) 84, 4184. 17. Huangfu, J., et al., Appl. Phys. Lett. (2004) 84, 1537. 18. Zhang, F. L., et al., IEEE Trans. Microw. Theory Tech. (2008) 56, 2566. 19. Enkrich, C., et al., Phys. Rev. Lett. (2005) 95, 203901. 20. Zhang, S., et al., Phys. Rev. Lett. (2005) 94, 037402. 21. Shalaev, V. M., et al., Opt. Lett. (2005) 30, 3356. 22. Zhou, X., and Zhao, X. P., Appl. Phys. Lett. (2007) 91, 181908. 23. Dolling, G., et al., Opt. Lett. (2006) 31, 1800. 24. Baena, J. D., et al., Appl. Phys. Lett. (2006) 88, 134108. 25. Gay-Balmaz, P., and Martin, O. J. F., Appl. Phys. Lett. (2002) 81, 939. 26. Koschny, T., et al., Phys. Rev. B (2005) 71, 21103. 27. Veselago, V. G., and Narimanov, E. E., Nat. Mater. (2006) 5, 759. 28. O’Brien, S., and. Pendry, J. B., J. Phys.: Condens. Matter (2002) 14, 4035.

61. Vendik, I. B., et al., Tech. Phys. Lett. (2006) 32, 429. 62. Ahmadi, A., and Mosallaei, H., Phys. Rev. B (2008) 77, 045104. 63. Yannopapas, V., Phys. Rev. B (2007) 75, 035112. 64. Kussow, A. G., et al., Phys. Stat. Sol. B (2008) 245, 992. 65. Kussow, A. G., et al., Phys. Rev. B (2007) 76, 195123. 66. Yannopapas, V., Appl. Phys. A (2007) 87, 259. 67. Qiu, C. W., and Gao, L., J. Opt. Soc. Am. B (2008) 25, 1728. 68. Yannopapas, V., Phys. Stat. Sol. (RRL) (2007) 1, 208. 69. Alu, A., and Engheta, N., J. Appl. Phys. (2005) 97, 094310. 70. Wheeler, M. S., et al., Phys. Rev. B (2006) 73, 045105. 71. Yannopapas, V., J. Phys.: Condens. Matter (2008) 20, 255201. 72. Gao, L., et al., Phys. Rev. E (2008) 78, 046609. 73. Alu, A., and Engheta, N., Phys. Rev. E (2005) 72, 016623. 74. Schuller, J. A., et al., Phys. Rev. Lett. (2007) 99, 107401.

29. Holloway, C. L., et al., IEEE Trans. Antennas Propag. (2003) 51, 2596.

75. Vynck, K., et al., “All-dielectric rod-type metamaterials operating at optical frequencies,” http://arxiv.org/abs/0805.0251 (2008).

30. Shalaev, V. M., Nat. Photon. (2007) 1, 41.

76. Fabre, N., et al., Phys. Rev. Lett. (2008) 101, 073901.

31. Padilla, W. J., et al., Materials Today (2006) 9, 28.

77. Gaillot, D. P., et al., Opt. Express (2008) 16, 3986.

32. Soukoulis, C. M., et al., Adv. Mater. (2006) 18, 1941.

78. Cai, W., et al., Opt. Express (2008) 16, 5444.

33. Engheta, N., and Ziolkowski, R. W., (eds.), Electromagnetic Metamaterials: Physics and Engineering Explorations, Wiley-IEEE Press, New Jersey, USA, (2006).

79. Chen, H. T., et al., Nature (2006) 444, 597.

34. Marques, R., Martin, F., and Sorolla, M., Metamaterials with Negative Parameters: Theory, Design, and Microwave Applications, Wiley-Interscience Press, New Jersey, USA, (2007).

80. Padilla, W. J., et al., Phys. Rev. Lett. (2006) 96, 107401. 81. Zhao, Q., et al., Appl. Phys. Lett. (2007) 90, 011112. 82. Zhang, F. L., et al., Appl. Phys. Lett (2008) 92, 193104.

35. Jackson, J. D., Classical Electrodynamics, 2nd ed., Wiley, New York, USA, (1999).

83. Hou, B., et al., Opt. Express (2005) 13, 9149.

36. Bohren, C. F., and Huffman, D. R., Absorption and Scattering of Light by Small Particles, Wiley-Interscience, New York, USA, (1983).

84. Huang, Y., et al., Prog. Nat. Sci. (2008) 18, 907.

37. Zhao, Q., et al., Phys. Rev. Lett. (2008) 101, 027402.

86. Kang, L., et al., Appl. Phys. Lett. (2008) 93, 171909.

38. Lewin, L., Proc. Inst. Electr. Eng. (1947) 94, 65.

87. Kang, L., et al., Opt. Express (2008) 16, 8825.

39. Jylha, L., et al., J. Appl. Phys. (2006) 99, 043102.

88. Kang, L., et al., Opt. Express (2008) 16, 17269.

40. Contopanagos, H. F., et al., J. Opt. Soc. Am. A (1999) 16, 1682.

89. Zhao, H. J., et al., Appl. Phys. Lett. (2007) 91, 131107.

41. Houzet, G., et al., Appl. Phys. Lett. (2008) 93, 053507.

90. Chen H., et al., Appl. Phys. Lett. (2006) 89, 053509.

42. Kittel, C., Introduction to Solid State Physics, 7th ed., John Wiley and Sons Inc., New York, USA, (1996).

91. Zhao, Q., et al., Appl. Phys. Lett. (2008) 92, 051106.

43. Popa, B.I., and Cummer, S.A., Phys. Rev. Lett. (2008) 100, 207401. 44. Acher, O., et al., Appl. Phys. Lett. (2008) 93, 032501. 45. Ueda, T., et al., IEEE Trans. Microw. Theory Tech. (2007) 55, 1280. 46. Lin, X. Q., et al., Appl. Phys. Lett. (2008) 92, 131904. 47. Ueda, T., et al., IEEE Trans. Microw. Theory Tech. (2008) 56, 2259. 48. Shibuya, K., et al., Terahertz metamaterials composed of TiO2 cube arrays, Presented at 2nd International Congress on Advanced Electromagnetic Materials in Microwaves and Optics, Pamplona, Spain, September 21-26, 2008.

85. Hand, T. H., and Cummer, S. A., J. Appl. Phys. (2008) 103, 066105.

92. Vendik, O. G., and Zubko, S. P., J. Appl. Phys. (1997) 82, 4475. 93. Gaillot, D. P., et al., New J. Phys. (2008) 10, 115039. 94. Khoo, I. C., et al., Opt. Lett. (2006) 31, 2592. 95. Gordon, J. A., and Ziolkowski, R. W., Opt. Express (2007) 15, 2622. 96. Huang, X. G., et al., Langmuir (2007) 23, 8695. 97. Li, W., et al., Langmuir (2008) 24, 13772.

DECEMBER 2009 | VOLUME 12 | NUMBER 12

69

Mie resonance-based dielectric metamaterials

Mie resonance-based dielectric metamaterials Increasing attention on metamaterials has been paid due to their exciting physical behaviors and potential applications. While most of such artificial material structures developed so far are based on metallic resonant structures, Mie resonances of dielectric particles open a simpler and more versatile route for construction of isotropic metamaterials with higher operating frequencies. Here, we review the recent progresses of Mie resonance-based metamaterials by providing a description of the underlying mechanisms to realize negative permeability, negative permittivity and double negative media. We address some potential novel applications. Qian Zhao1,2, Ji Zhou1,*, Fuli Zhang3, Didier Lippens3 1 State Key Lab of New Ceramics and Fine Processing, Department of Materials Science and Engineering, Tsinghua University, Beijing, PRC 2 State Key Lab of Tribology, Department of Precision Instruments and Mechanology, Tsinghua University, Beijing, PRC 3 Institut d’Electronique de Micro-électronique et de Nanotechnologie, UMR CNRS 8520, University of Lille 1, Villeneuve d’Ascq Cedex, France *E-mail: [email protected]

Metamaterials are artificial electromagnetic media structured on

opening the effective parameter space, so that new functionalities

a scale much shorter than their operating wavelength. Under this

in the light scattering can be envisaged.

condition they can be considered as homogeneous media whose

values of the effective permittivity and permeability was also

than periodic effects as it is the case for photonic crystal or more

recognized as one of the major goals of this research area. Great

generally electromagnetic band gap material. Their basic cells

progress in electromagnetic metamaterials has been achieved for

are generally constituted of resonant inclusions which yield a π

these unique physical properties and novel potential applications,

phaseshift in the material response above the resonant frequency.

such as negative refraction2, 3, perfect lens4, 5 and cloaking6-8 have

As a consequence, their effective permittivity and permeability

been shown. They have been experimentally demonstrated in a

can be negative either in separate or overlapping frequency

frequency range from the radio frequencies9 to millimeter waves10,

bands, a unique and distinct property that is not observed in

infrared wavelengths11-13, and visible optics14. Up to date, most

naturally occurring

materials1

. For the latter condition they can

be considered as double negative or negative index media hence

60

Also recently, the achievement of near-zero or less than unity

electromagnetic properties rely mainly on the basic cell rather

DECEMBER 2009 | VOLUME 12 | NUMBER 12

of metamaterials are constructed with the use of sub-wavelength resonant metallic elements. For instance, the first left-handed

ISSN:1369 7021 © Elsevier Ltd 2009

Mie resonance-based dielectric metamaterials

(a)

(b)

(c)

(d)

REVIEW

Fig. 1 Electric and magnetic field distribution in a dielectric cube with the magnetic field polarized along the z axis and electric field polarized along the y axis. (a) Electric field in the plane z=0 near the first Mie resonance. (b) Magnetic field in the plane y=0 near the first Mie resonance. (c) Electric field in the plane z=0 near the second Mie resonance. (d) Magnetic field in the plane y=0 near the second Mie resonance. (Reprinted with permission from37. © 2008 American Physical Society.)

metamaterials (LHMs) with simultaneously negative permittivity and

Mie resonance of particles

permeability have been fabricated by means of metallic split ring

From the viewpoint of scattering theory, all scattering objects can

resonators (SRRs) and wires15, 16, for tailoring the magnetic and electric

be represented by effective electric and/or magnetic polarizability

responses, respectively. Other metallic elements, such as Ω-shaped

densities. Light scattering by small (relative to the incident light

structures17, 18, U-shaped structures19, staplelike structures20, paired

wavelength) spherical particles is a fundamental topic in classical

rods21, dendritic22 and fishnet structures23, are also successfully used

electrodynamics35, and is based upon the exact Mie solution of the

to fabricate LHMs.

diffraction problem36. The scattered field of a single isolated dielectric

Usually, the metallic constitutive elements have conductive loss and

sphere with radius r0 and relative refractive index n can be decomposed

anisotropic electromagnetic responses. Several authors have suggested

into a multipole series with the 2m-pole term of the scattered electric

methods24-26 to construct isotropic metamaterials by combining

field proportional to

metallic SRRs and wires. However it is difficult to fabricate the bulk arrays of complex geometry with submicron or nanoscale sizes in

am =

order to generate a negative permeability effect at infrared and optical frequencies27. Recently, another route based on the interaction between

dielectric inclusions provide a novel mechanism for the creation of magnetic or electric resonance based on displacement currents, and

(1)

whereas the 2m-pole term of the scattered magnetic field is proportional to

electromagnetic waves and dielectric particles28, 29 was proposed to achieve the electric or magnetic resonances. The Mie resonances of

nψ m (nx)ψ m' ( x) − ψ m ( x)ψ m' (nx) nψ m (nx)ξ m' ( x) − ξ m ( x)ψ m' (nx)

bm =

ψ m (nx)ψ m' ( x) − nψ m ( x)ψ m' (nx) ψ m (nx)ξ m' ( x) − nξ m ( x)ψ m' (nx)

(2)

where x=k0r0, k0 is the free-space wavenumber, and ψm(x) and

offer a simpler and more versatile route for the fabrication of isotropic

ξm(x) are the Riccati-Bessel functions. The primes indicate derivation

metamaterials operating at higher frequencies. The progress on metallic

with respect to the arguments. The scattering coefficient am and

elements-based metamaterials has been reviewed in many articles30-32

bm are related to the electric and magnetic responses of the sphere,

and books33, 34. In this review, we focus on the scattering mechanisms

respectively. From the Mie theory we can calculate the electric and

based on Mie resonance in dielectric particles and describe the recent

magnetic dipole coefficients, a1 and b1, respectively. From effective

progress in these metamaterials including ferroelectric and polaritonic

medium theory, we know that these are the multipole terms which

particles and their tunable behaviors.

contribute most significantly to the effective permittivity and

DECEMBER 2009 | VOLUME 12 | NUMBER 12

61

REVIEW

Mie resonance-based dielectric metamaterials

μ eff

⎛ ⎜ 3v f = μ 1 ⎜1 + ⎜ F (θ ) + 2bm −vf ⎜ F (θ ) − bm ⎝

⎞ ⎟ ⎟ ⎟ ⎟ ⎠

(4)

where

F (θ ) =

2(sin θ − θ cosθ ) (θ 2 − 1) sin θ + θ cosθ

be = ε 1 ε 2 , bm = μ1 μ 2

(5)

(6)

The volume fraction of the spherical particles,

4 r v f = π ( 0 ) 3 , θ = k 0 r0 ε 2 μ 2 , r0 and p are the particle radius and 3 p Fig. 2 Calculated effective permittivity εeff and permeability μeff of the magnetodielectric sphere arrays composite. (Reprinted with permission from29. © 2003 IEEE.)

the lattice constant, respectively. Eq 5 shows that F(θ) is a resonant

permeability of the particle composite. Since the magnetic response of

values of F(θ) with a magnitude on the order of unity as given by

a nonmagnetic particle is usually weak, it is important to strengthen

Eqs. (3) and (4).

function and becomes negative above resonance in some range of θ, resulting in the negative permittivity or permeability for negative

In Lewin’s model, the constitutive parameters were formulated

the electromagnetic resonant behavior. For the lowest resonant frequencies of a1 and b1, the sphere exhibits electric and magnetic

only considering the spheres resonating either in the first or second

dipoles. This conclusion can be assessed from the electromagnetic

resonant modes of the Mie series. This is because the higher order Mie

intensity distributions in a high dielectric ceramic cube for a plane

resonances often occur at frequencies beyond the long wavelength

incident wave propagating along the x axis37 (Fig. 1). It can be seen

limit, and thus the Clausius-Mossotti equation does not apply. Then,

that the electric or magnetic fields are mainly localized in the cubes.

Jylha et al.39 improved those formulations by taking into account the

The azimuthal component of the displacement current inside each

electric polarizabilities of spheres operating in the magnetic resonant

cube is greatly enhanced at the first Mie resonance (Fig. 1a) resulting

modes. Independent of Lewin’s model, O’Brien and Pendry28 showed that a

in a large magnetic field along the z axis (Fig. 1b) which corresponds to the TE011 Mie resonance mode. At the second Mie resonance, the

negative effective permeability can be obtained in a two-dimensional

y component of the displacement current inside the cubes increases

array of ferroelectric rods with the magnetic field polarized along the

dramatically (Fig. 1c) and hence with a large magnetic field along

axes of the rods. Although the underlying physics is the same, the

the azimuth (Fig. 1d), which corresponds to the TM011 Mie resonance

authors used another method40 (transfer matrix method) to find the

mode.

effective media values with similar conclusion. The aforementioned

These electric and magnetic dipole resonances act as artificial

theoretical results show that a high permittivity microstructured

‘atoms’ which form the basis of new optical materials. In a material

medium can exhibit isotropic negative values of the effective

made up of a collection of such resonant particles, their combined

permeability and permittivity.

scattering response can act like a material with almost arbitrary values of effective permittivity and permeability. This idea can be verified by using the model proposed in 1947 by

Lewin38

who considered the

electromagnetic scattering properties of a composite material which

With the rapid development of LHMs, Lewin’s model was reconsidered

was constituted of an array of lossless magnetodielectric spheres (ε2

and introduced into the realm of metamaterials to realize single and

and μ2) embedded in another background matrix (ε1 and μ1). The

double negative media. Based on Lewin’s model, Holloway et al.29

effective permittivity εeff and permeability μeff expressions based on

numerically demonstrated the feasibility of achieving simultaneously negative εeff and μeff in the magnetodielectric sphere arrays for

Mie theory are as follows38.

ε eff

62

Mie resonance as a new route for metamaterials

⎛ ⎜ 3v f = ε 1 ⎜1 + ⎜ F (θ ) + 2be −vf ⎜ F (θ ) − be ⎝

⎞ ⎟ ⎟ ⎟ ⎟ ⎠

DECEMBER 2009 | VOLUME 12 | NUMBER 12

wavelengths where the electric and magnetic resonances are excited in the spheres. Eqs. (3) and (4) show that εeff and μeff depend on the (3)

permeability and permittivity of the dielectric inclusions and host medium, as well as the volume fraction of spheres of radius r0. Fig. 2 shows εeff and μeff calculated for υf = 0.5, ε1 = μ1 = 1, ε2 = 40, and

Mie resonance-based dielectric metamaterials

REVIEW

μ2 = 200 as a function of k0r0. There are two regions where both εeff and μeff become negative with the bandwidths becoming narrower by

(a)

decreasing the volume fraction υf. From a practical point of view, many kinds of materials and shapes of particles have been proposed in the literature to fabricate negative or less than unity permeability and permittivity dielectric metamaterials operating in different frequency regions. The designing ideas are summarized in the following.

Magnetic response The realization of abnormal permeability is a tricky issue for various metamaterials, because the magnetic response of materials is usually

(b)

weak, especially at infrared or visible frequencies. Lewin’s model shows that two methods based on Mie resonance can be used to achieve a negative effective permeability effect. The first one is to use magnetodielectric inclusions with large values of permeability and permittivity. The second method is to use nonmagnetic dielectric particles with extremely large permittivity values. In the former case, two terms be and bm in Eqs. (3) and (4) contribute to the negative permeability, while only be plays an important role for the latter. The possibility to use magnetodielectric particles has been numerically demonstrated29. However a magnetodielectric particle with

(c)

simultaneously large values of permittivity and permeability seems physically unattainable even in the microwave. Eq. (4) indicates that nonmagnetic spheres with very high permittivity values can also be employed to induce negative permeability and permittivity effects at the different Mie resonance frequencies. Polaritonic materials, such as ionic solids and polar semiconductors, or ferroelectric materials can provide the large permittivity. For ferroelectric materials, their extreme high permittivity values can be preserved at least up to millimeter wavelengths41. At infrared frequencies however a roll-off of the dielectric constant is observed so that they cannot be used in this frequency range. In contrast, the lattice resonance in polaritonic crystals can be exploited to tailor the permittivity resonance at infrared and optical frequencies. As a consequence, the polaritonic resonance of crystals could be potentially used in the infrared spectral region. The relative permittivity is42

⎛ ⎞ ω2 −ω2 ⎟⎟ , ε r (ω ) = ε (∞)⎜⎜1 + 2 L 2 T ω − ω − i ω γ T ⎝ ⎠

Fig. 3 A three-dimensional dielectric composite with isotropic negative permeability. (a) Photograph of BST cubes arrayed in Teflon substrate. (b) Transmission for the dielectric cube array only (dashed line), wire array only (dotted line), and the combination of BST cubes and wires (solid line). Inset of Fig. 3(b) shows the measured and calculated transmission phase. (c) Retrieved refractive index and permeability (inset). (Reprinted with permission from37. © 2008 American Physical Society.)

experimentally demonstrated in the microwave region37. The dielectric (7)

where ε(∞) is the high-frequency limit of the permittivity, ωT and

cube side length l was 1.0 mm for a lattice constant of 2.5 mm. And the first TE and TM resonance modes, i.e., magnetic and electric resonances were determined by transmission measurements at 6.12

ωL are the transverse and longitudinal optical phonon frequencies, and

and 8.28 GHz respectively. Using smaller cubes (l =0.75 mm) with

γ is the damping coefficient. Therefore, large values of εr(ω) can be

a magnetic resonance near 8.5 GHz, in conjunction with an electric

achieved near the transverse phonon frequency.

response from metallic wires, researchers fabricated double negative

A three-dimensional dielectric composite consisting of an array

media. The results of transmission measurements are displayed in

of dielectric cubes [Ba0.5Sr0.5TiO3 (BST)] with a relative permittivity

Fig. 3b and the retrieved electromagnetic parameters (Fig. 3c) further

of 1600 in a Teflon substrate was fabricated (Fig. 3a) to demonstrate

verified the negative permeability near the first Mie resonance.

the feasibility of this full dielectric metamaterial route. On this basis, isotropic negative values of the effective permeability were

A rectangular dielectric block43 and piezoelectric disks44 were also experimentally verified to design very low-loss magnetic metamaterials.

DECEMBER 2009 | VOLUME 12 | NUMBER 12

63

REVIEW

Mie resonance-based dielectric metamaterials

(a)

(b)

Fig. 4 Schematic of metamaterials based on Mie resonance. (a) A two-dimensional lattice structure for one dielectric-resonator in the cutoff microwave waveguide. (Reprinted with permission from45. © 2007 IEEE.) (b) Terahertz metamaterial consisting of polycrystalline TiO2 cubes-arrays on the Al2O3 substrate. (Reprinted with permission from48. © 2008 Metamaterials.)

Also a two-dimensional square lattice of dielectric disk inserted between two metallic parallel-plate waveguide (Fig. 4a) was also used

(a)

to demonstrate negative refraction, where the macroscopic behavior of dielectric disk provides negative effective permeability and the waveguide plays a role in a TE cut-off waveguide leading to negative effective permittivity45. A dielectric block [(Zr,Sn)TiO4 ceramics, dielectric constant 36.7] with a thin metallic rod screwed inside was proposed to fabricate gradient metamaterial lenses and numerically demonstrated to deflect and focus the incident plane waves46. Dielectric-resonator-based composite right/left-handed transmission lines used to the design of leaky wave antenna can alleviate the significantly large conducting loss and increase the radiation efficiency47. Terahertz metamaterials based

(b)

on the Mie resonance of polycrystalline TiO2 cubes-arrays on the Al2O3 substrate (Fig. 4b) were also experimentally demonstrated by Shibuya et al.48, in which the negative permeability and permittivity occur around 0.28 and 0.38 THz, respectively. A three-dimensional collection of polaritonic spheres was proposed to obtain isotropic negative effective permeability near the first Mie resonance at infrared frequencies49. The calculated effective parameters (LiTaO3 crystal) reported in this reference are shown in Fig. 5 and the isotropy of electromagnetic properties was also verified by a comparison with a full multiple scattering approach. Semiconductor nanoparticles, such as CuCl with a Z3 exciton line at 386.93 nm, Cu2O

Fig. 5 The calculated effective relative permeability (a) and permittivity (b) of a collection of LiTaO3 spheres. (Reprinted with permission from49. © 2005 American Physical Society.)

with a 2P exciton50, and GaP51 were also suggested to realize negative permeability within and below the optical region. Metal nanoclusters

64

Similar to spherical or cubic dielectric elements, the cylindrical

possessing large permittivity at visible frequency can also be used to

particles can also generate the Mie electromagnetic resonances.

obtain magnetic Mie resonance52, 53.

The most important issue is to determine the resonant modes. For

DECEMBER 2009 | VOLUME 12 | NUMBER 12

Mie resonance-based dielectric metamaterials

REVIEW

Pendry et al.59 suggested a metallic wire array structure to realize a

a TE polarization (E field perpendicular to the rod axis), the lowest Mie resonance mode (TE0) corresponds to the magnetic response,

plasma-like state. With such a configuration, the negative permittivity

resulting in negative permeability values. A two-dimensional array of

frequency range can be tuned by the lattice constant and the wire

ferroelectric rods28, 54 and polaritonic rods55 were proposed to obtain

diameter in the low frequency spectral region even at microwave

negative effective permeability56, which can be considered as the

frequencies. Additionally, negative dielectric permittivity can also be

TE0 mode. For TM polarization (E field parallel to the rod axis), the

obtained in more ordinary dielectric media with bound charges, within

lowest two Mie resonances modes, TM0 and TM1, correspond to the

a frequency band above a resonance frequency, where the resonant

electric and magnetic responses, and consequently lead to negative

Lorentz permittivity occurs58.

permittivity and permeability, respectively. The electromagnetic field

Another method is to use the electric resonant mode of the Mie

distribution displayed for the TM1 mode (Fig. 6) can further clarify the

resonance of dielectric particles. For the dielectric sphere or cube, it can

magnetic resonance mechanism57. The electric field is distributed along

be equivalent to a dipole at the second resonant mode as exemplified

the ± z directions with opposite signs along the propagation direction

by the field mapping shown in Fig. 1. For a dielectric column particle,

(Fig. 6b), accounting for a strong circular displacement current (Fig. 6d).

it can be equivalent to an electric dipole at the first resonance mode

Such displacement current results in a large magnetic field along the y

(TM0) and can result in negative permittivity.

axis (Fig. 6c), which corresponds to the TM1 mode.

Negative refraction Electric response

The mechanisms of electric and magnetic resonances in dielectric

An electric response can be accomplished with simpler metallic

particles (spheres, cubes or rods) have been analyzed above. Negative

structures, such as uncoupled rods or strips. The first method to

refraction can be fulfilled by combing the two resonances together.

obtain negative permittivity is the bulk metals at optical frequencies,

However, the first electric resonance (TM mode) is at a higher

where conduction electrons can be assumed to be reasonably free and

frequency than the fundamental magnetic resonance (TE mode) for

plasma-like behavior is responsible for a negative dielectric permittivity

the identical sphere. Due to the different resonance frequencies of TE

at frequencies less than the plasma

frequency58.

Usually, the plasma

and TM modes in the different-sized particles, we can consider the

frequencies of metals are at ultraviolet frequencies and dissipation is

conditions when the first lowest resonance of TM011 mode related

small. As the frequency is much lower than the plasma frequency, the

to a bigger sphere coincides with the TE011 resonance in a smaller

imaginary part of the complex permittivity increases dramatically while

sphere. Recently, Vendik et al.60, 61 numerically studied an artificial

very large negative values of the real part are obtained.

double negative media whose basic unit cell is composed by two

(a)

(b)

(c)

(d)

Fig. 6 Electric and magnetic field distributions in a dielectric rod at the second resonant mode (TM1 mode). (a) Unit cell configuration. (b) Electric field distribution. (c) Magnetic field distribution. (d) Equivalent current ring. (Reprinted with permission from57. © 2007 American Physical Society.)

DECEMBER 2009 | VOLUME 12 | NUMBER 12

65

REVIEW

Mie resonance-based dielectric metamaterials

dielectric spheres of different sizes. The larger sphere was used for the negative permittivity while the small one allows achieving a negative

(a)

permeability in the same microwave frequency band. At the same time, two sets of spheres, having the same size but different materials, were also developed to realize negative refraction62. More recently, a threedimensional isotropic negative-index composite at infrared or visible frequencies was reported51, 63-66. The proposed homogeneous isotropic structures consist of dielectric spheres (gallium phosphide) embedded randomly in a negative permittivity host medium (Cesium)51, or two interpenetrating lattices of spheres63-66. One lattice ensures a negative permeability using a polaritonic material (LiTaO3, SiC, CuCl) and the other lattice creates a negative permittivity effect by using a plasmonic

(b)

material (n-type Ge, Au, MgB2). Negative refraction index effect exists not only in the situation of a regular lattice arrangement but also for randomly distributed nanoparticles when the losses are ignored. However, the numerical results also demonstrated that the negative refraction could not be achieved owing to the large imaginary part of the wave vector corresponding to evanescent rather than propagating waves when the losses of the constitutive materials were taken into account. Another method to fabricate isotropic LHMs based on Mie resonance is using only one kind of micron-scale non-magnetic coated

spheres67-69.

(c)

The underlying physical mechanisms correspond

to a negative effective permeability effect due to polaritonic sphere core while a negative effective permittivity effect results from an electric-dipole resonance of sphere coating on its outer surface whose dispersion follows a Drude model. For an isolated sphere, an electric dipole resonance can be driven when its material permittivity is -2. Since this permittivity value is negative, the electric field is evanescent within the sphere so that such electric dipole resonance is a surface resonance in contrast to the volume effect of the magnetic resonance. Therefore, the coating can be designed to have a negative permittivity. Note that the magnetic resonance of the core is hardly affected, as long as the permittivity of the coating remains small

Fig. 7 The effective (a) permeability, (b) permittivity, and (c) index of a collection coated spheres. The cores are made of LiTaO3 with radius 4 μm, and the coatings are a Drude material with radius 0.7 μm. (Reprinted with permission from70. © 2006 American Physical Society.)

in comparison to the large permittivity of the core. The spheres with a core of a polaritonic crystal LiTaO3 and the coated thin layer

resonance modes of SiC particles at mid-IR under various polarization

of a Drude model semiconductor (or a polaritonic material) were

conditions. Also they proposed to obtain a negative refractive index by

used to demonstrate isotropic negative refraction70. The calculated

combining the two resonances of TM0 and TM1 modes (Fig. 8).

effective electromagnetic parameters are shown in Fig. 7. Such three-

rods in s-polarized light was presented recently. The authors claimed

can be used to realize subwavelength imaging71 and electromagnetic

that large wavelength-to-period ratios do not necessarily result in an

transparency72, 73.

isotropic metamaterial. They also suggested that silicon rod arrays

Besides dielectric spheres array, the electric and magnetic Mie

66

A theory on the electric and magnetic dipole activities of dielectric

dimensional LHMs consisting of metal-coated semiconductor spheres

could exhibit a true metamaterial left handed dispersion branch in

resonances in dielectric rods can also be used to achieve negative

the visible to mid-IR despite the moderate value of the refractive

permittivity and permeability values. Under TM illumination, a

index (n~3.5)75. Such a conclusion is interesting by considering Mie

resonant permittivity due to the TM0 mode excitation and a resonant

resonance in moderate permittivity materials in optics. It has however

permeability due to the TM1 mode excitation can be used to realize

to be checked by experiments in order to discriminate negative

negative permittivity and permeability, respectively. Schuller et al.74

refraction effects resulting from the conventional band folding in

experimentally and numerically observed and identified the Mie

the diffraction regime76 from pure left handed branch effects in the

DECEMBER 2009 | VOLUME 12 | NUMBER 12

Mie resonance-based dielectric metamaterials

REVIEW

(a)

(b)

Fig. 10 Schematic of a cylindrical non-magnetic cloak for TE polarization at mid-infrared. (Reprinted with permission from78. © 2008 Optical Society of America.)

waves and realize invisibility cloak6. Effective permeability can be less than unity around the magnetic resonance and such metamaterials have been suggested to construct invisibility cloak7, 8. An all-dielectric Fig. 8 (a) Calculated effective permeability for a normal incidence TE illuminated array of infinitely long SiC rods. (b) Calculated permittivity (permeability) due to excitation of the zeroth (first) order TM mode. (Reprinted with permission from74. © 2007 American Physical Society.)

cloak (Fig. 9) consisting of radially positioned micrometer-sized ferroelectric cylinders was suggested to perform cloaking at 0.58 THz, which exhibits a strong magnetic resonance based on Mie theory77. At last, Silicon Carbide (SiC) rod, a polaritonic material with phonon resonance bands centered around 12.5 μm, was also suggested to built

(a)

(b)

transparency cloak (Fig. 10) at mid-infrared with the TE resonance mode78. To sum up, an all-dielectric configuration provides an attractive route for designing cloaking devices at microwave, terahertz and infrared frequencies.

Tunable Mie resonance-based metamaterials (c)

(d)

As seen in the previous sections, resonance effects in the electric and magnetic responses appear as a necessary condition for fabricating left-handed metamaterials. Such resonances are strongly dependent on the geometrical dimensions and on the dielectric properties of the constitutive elements. Usually negative values can only be achieved over a narrow frequency range near the resonances, especially for the

Fig. 9 (a) Schematic of a terahertz all-dielectric cloak. Steady-state Ez pattern calculated at 0.58 THz for a copper rod without (b) and with cloak (c). (d) Magnified view of the field pattern of (c). (Reprinted with permission from77. © 2008 Optical Society of America.)

magnetic resonance. From the application point of view, and for a deeper understanding of the intrinsic properties of negative media, it is desirable to implement structures with tunable and reconfigurable resonant properties79. Some tunable metamaterials based on the

long wavelength regime. A verification of negative refraction in a TM

metallic structures have been proposed by modifying the locally

illuminated array of large permittivity ceramic rods was experimentally

dielectric or permeability environment. For example, a control of the

verified at microwave frequencies, corresponding to the combination of

electric and magnetic responses of SRRs and related configurations was

TM0 and TM1 modes57.

experimentally demonstrated through photoexcitation of free carriers in a GaAs substrate80, electrically or magnetically controlled liquid

All-dielectric cloaks

crystals81, 82, along with electrorehological fluids83, 84, ferroelectric85,

Conformal transformation of electromagnetic domains has been

ferromagnetic materials86-89 and other methods90. All these examples

proposed as an exciting approach to control the flow of propagating

correspond however to anisotropic tunable metamaterials whereas

DECEMBER 2009 | VOLUME 12 | NUMBER 12

67

REVIEW

Mie resonance-based dielectric metamaterials

the sample temperature. For a proof of this principle, a simple cubic lattice of ceramic cubes of 0.45 mm side length (BST doped with 5wt% MgO) were arrayed in a Teflon substrate with a lattice constant of 1.25 mm. The microwave scattering parameters were measured under various temperature conditions (Fig. 11a, b). The magnetic resonance corresponding to the first Mie resonance in the dielectric cubes can be continuously and reversibly adjusted from 13.65 GHz to 19.28 GHz (a)

with a temperature changing from -15˚C to 35˚C. The frequency dependence of the effective permeability, displayed in Fig. 11c, shows that negative permeability values can be achieved in a frequency band of about 6 GHz by a temperature variation of 50˚C. It is believed that this temperature controlled metamaterial could be used for the design of adaptive three-dimensional metamaterials and invisibility cloaks which exhibit basically a very narrow fractional bandwidth of the order of 1%93. Another method used to adjust the negative refraction of Mie resonance is to alter the dielectric property of the background medium. Khoo et al.94 proposed nanospheres dispersed liquid crystals to realize

(b)

tunable negative–zero–positive index of refraction in the optical and terahertz regimes.

Outlook As an alternative method for the design of electromagnetic metamaterials, the dielectric particles show several advantages, notably in terms of isotropic parameters, and the fabrication techniques targeting at higher frequencies of operation. Although several experimental demonstrations have allowed the verification of the first principles at microwave and terahertz frequencies, it appears that the research on this area is at a very primary stage with numerous (c)

theoretical and numerical studies. Further experimental works are expected at mid-term in order to demonstrate the possibility of fabricating isotropic negative index material notably in the infrared and visible frequency ranges. Towards this goal the challenging issues

Fig. 11 The actively modulated isotropic negative permeability dielectric composite. (a) Dependence of the first magnetic resonance on the temperature. (b) Dependence of transmission phases on the temperature. (c) Calculated effective permeability under different temperature. (Reprinted with permission from91. © 2008 American Institute of Physics.)

are the preservation of large dielectric constant and low loss in these frequency ranges, which appear as the necessary condition to operate in the long wavelength regime. The introduction of active materials may alleviate or even overcome the problem of intrinsic losses95. At last the inexpensive chemical methods, such as colloidal crystallization,

isotropic properties can be more suitable for potential applications

may be suitable for the synthesis of nanoparticles96, 97. Although much

notably for all angle negative refraction.

work is needed before practical implementations are possible, dielectric

The first dynamic tuning of isotropic metamaterial relying on Mie resonance has been demonstrated recently by altering the dielectric property of the basic

cell91.

As expected from the Mie resonance

metamaterials are a promising candidate for real-world application of the many exciting opportunities provided by electromagnetic metamaterials.

theory, at the first resonance the dielectric sphere is equivalent to a magnetic dipole with a resonance frequency ω ≈ πc /(r0 ε 2 )

Acknowledgments

within the long-wavelength limit. Usually, the permittivity of the

This work is supported by the National Science Foundation of China under Grant Nos. 50425204, 50621201, 50632030, 60608016 and 10774087, and by the State Key Lab of Tribology under Grant No. SKLT 08B12. D.L. would like also to thank the Delegation Générale pour l’Armement for its support in the framework of the contract 06.34.021.

high κ ceramic inclusions varies as a function not only of the local field, but also of temperature92. Therefore, a variation of the effective permeability of the composite material can be realized by changing

68

DECEMBER 2009 | VOLUME 12 | NUMBER 12

Mie resonance-based dielectric metamaterials

REVIEW

Reference 1. Pendry, J. B., Nature Mater. (2006) 5, 763.

49. Wheeler, M. S., et al., Phys. Rev. B (2005) 72, 193103.

2. Shelby, R. A., et al., Science (2001) 292, 77.

50. Yannopapas, V., and Vitanov, N. V., Phys. Rev. B (2006) 74, 193304.

3. Houck, A. A., et al., Phys. Rev. Lett. (2003) 90, 137401.

51. Seo, B. J., et al., Appl. Phys. Lett. (2006) 88, 161122.

4. Pendry, J. B., Phys. Rev. Lett. (2000) 85, 3966.

52. Wu, Q., and Park, W., Appl. Phys. Lett. (2008) 92, 153114.

5. Fang, N., et al., Science (2005) 308, 534.

53. Rockstuhl, C., et al., Phys. Rev. Lett. (2007) 99, 017401.

6. Pendry, J. B., et al., Science (2006) 312, 1780.

54. Felbacq, D., and Bouchitte, G., New J. Phys. (2005) 7, 159.

7. Schurig, D., et al., Science (2006) 314, 977.

55. Huang, K. C., et al., Appl. Phys. Lett. (2004) 85, 543.

8. Cai, W., et al., Nat. Photonics (2007) 1, 224.

56. Felbacq, D., and Bouchitte, G., Phys. Rev. Lett. (2005) 94,183902.

9. Wiltshire, M. C. K., et al., Science (2001) 291, 849.

57. Peng, L., et al., Phys. Rev. Lett. (2007) 98, 157403.

10. Zhang, F. L., et al., Appl. Phys. Lett. (2008) 93, 083104.

58. Ramakrishna, S. A., Rep. Prog. Phys. (2005) 68, 449.

11. Dolling, G., et al., Science (2006) 312, 892.

59. Pendry, J. B., Phys. Rev. Lett. (1996) 76, 4773.

12. Linden, S., et al., Science (2004) 306, 1351.

60. Vendik, O. G., and Gashinova, M. S., in Proceedings of the 34th European Microwave Conference, Amsterdam (IEEE Press, Piscataway, NJ, 2004), Vol. 3, pp. 1209-1212.

13. Liu, H., et al., Adv. Mater. (2008) 20, 2050. 14. Dolling, G., et al., Opt. Lett. (2007) 32, 53. 15. Pendry, J. B., et al., IEEE Trans. Microw. Theory Tech. (1999) 47, 2075. 16. Smith, D. R., et al., Phys. Rev. Lett. (2000) 84, 4184. 17. Huangfu, J., et al., Appl. Phys. Lett. (2004) 84, 1537. 18. Zhang, F. L., et al., IEEE Trans. Microw. Theory Tech. (2008) 56, 2566. 19. Enkrich, C., et al., Phys. Rev. Lett. (2005) 95, 203901. 20. Zhang, S., et al., Phys. Rev. Lett. (2005) 94, 037402. 21. Shalaev, V. M., et al., Opt. Lett. (2005) 30, 3356. 22. Zhou, X., and Zhao, X. P., Appl. Phys. Lett. (2007) 91, 181908. 23. Dolling, G., et al., Opt. Lett. (2006) 31, 1800. 24. Baena, J. D., et al., Appl. Phys. Lett. (2006) 88, 134108. 25. Gay-Balmaz, P., and Martin, O. J. F., Appl. Phys. Lett. (2002) 81, 939. 26. Koschny, T., et al., Phys. Rev. B (2005) 71, 21103. 27. Veselago, V. G., and Narimanov, E. E., Nat. Mater. (2006) 5, 759. 28. O’Brien, S., and. Pendry, J. B., J. Phys.: Condens. Matter (2002) 14, 4035.

61. Vendik, I. B., et al., Tech. Phys. Lett. (2006) 32, 429. 62. Ahmadi, A., and Mosallaei, H., Phys. Rev. B (2008) 77, 045104. 63. Yannopapas, V., Phys. Rev. B (2007) 75, 035112. 64. Kussow, A. G., et al., Phys. Stat. Sol. B (2008) 245, 992. 65. Kussow, A. G., et al., Phys. Rev. B (2007) 76, 195123. 66. Yannopapas, V., Appl. Phys. A (2007) 87, 259. 67. Qiu, C. W., and Gao, L., J. Opt. Soc. Am. B (2008) 25, 1728. 68. Yannopapas, V., Phys. Stat. Sol. (RRL) (2007) 1, 208. 69. Alu, A., and Engheta, N., J. Appl. Phys. (2005) 97, 094310. 70. Wheeler, M. S., et al., Phys. Rev. B (2006) 73, 045105. 71. Yannopapas, V., J. Phys.: Condens. Matter (2008) 20, 255201. 72. Gao, L., et al., Phys. Rev. E (2008) 78, 046609. 73. Alu, A., and Engheta, N., Phys. Rev. E (2005) 72, 016623. 74. Schuller, J. A., et al., Phys. Rev. Lett. (2007) 99, 107401.

29. Holloway, C. L., et al., IEEE Trans. Antennas Propag. (2003) 51, 2596.

75. Vynck, K., et al., “All-dielectric rod-type metamaterials operating at optical frequencies,” http://arxiv.org/abs/0805.0251 (2008).

30. Shalaev, V. M., Nat. Photon. (2007) 1, 41.

76. Fabre, N., et al., Phys. Rev. Lett. (2008) 101, 073901.

31. Padilla, W. J., et al., Materials Today (2006) 9, 28.

77. Gaillot, D. P., et al., Opt. Express (2008) 16, 3986.

32. Soukoulis, C. M., et al., Adv. Mater. (2006) 18, 1941.

78. Cai, W., et al., Opt. Express (2008) 16, 5444.

33. Engheta, N., and Ziolkowski, R. W., (eds.), Electromagnetic Metamaterials: Physics and Engineering Explorations, Wiley-IEEE Press, New Jersey, USA, (2006).

79. Chen, H. T., et al., Nature (2006) 444, 597.

34. Marques, R., Martin, F., and Sorolla, M., Metamaterials with Negative Parameters: Theory, Design, and Microwave Applications, Wiley-Interscience Press, New Jersey, USA, (2007).

80. Padilla, W. J., et al., Phys. Rev. Lett. (2006) 96, 107401. 81. Zhao, Q., et al., Appl. Phys. Lett. (2007) 90, 011112. 82. Zhang, F. L., et al., Appl. Phys. Lett (2008) 92, 193104.

35. Jackson, J. D., Classical Electrodynamics, 2nd ed., Wiley, New York, USA, (1999).

83. Hou, B., et al., Opt. Express (2005) 13, 9149.

36. Bohren, C. F., and Huffman, D. R., Absorption and Scattering of Light by Small Particles, Wiley-Interscience, New York, USA, (1983).

84. Huang, Y., et al., Prog. Nat. Sci. (2008) 18, 907.

37. Zhao, Q., et al., Phys. Rev. Lett. (2008) 101, 027402.

86. Kang, L., et al., Appl. Phys. Lett. (2008) 93, 171909.

38. Lewin, L., Proc. Inst. Electr. Eng. (1947) 94, 65.

87. Kang, L., et al., Opt. Express (2008) 16, 8825.

39. Jylha, L., et al., J. Appl. Phys. (2006) 99, 043102.

88. Kang, L., et al., Opt. Express (2008) 16, 17269.

40. Contopanagos, H. F., et al., J. Opt. Soc. Am. A (1999) 16, 1682.

89. Zhao, H. J., et al., Appl. Phys. Lett. (2007) 91, 131107.

41. Houzet, G., et al., Appl. Phys. Lett. (2008) 93, 053507.

90. Chen H., et al., Appl. Phys. Lett. (2006) 89, 053509.

42. Kittel, C., Introduction to Solid State Physics, 7th ed., John Wiley and Sons Inc., New York, USA, (1996).

91. Zhao, Q., et al., Appl. Phys. Lett. (2008) 92, 051106.

43. Popa, B.I., and Cummer, S.A., Phys. Rev. Lett. (2008) 100, 207401. 44. Acher, O., et al., Appl. Phys. Lett. (2008) 93, 032501. 45. Ueda, T., et al., IEEE Trans. Microw. Theory Tech. (2007) 55, 1280. 46. Lin, X. Q., et al., Appl. Phys. Lett. (2008) 92, 131904. 47. Ueda, T., et al., IEEE Trans. Microw. Theory Tech. (2008) 56, 2259. 48. Shibuya, K., et al., Terahertz metamaterials composed of TiO2 cube arrays, Presented at 2nd International Congress on Advanced Electromagnetic Materials in Microwaves and Optics, Pamplona, Spain, September 21-26, 2008.

85. Hand, T. H., and Cummer, S. A., J. Appl. Phys. (2008) 103, 066105.

92. Vendik, O. G., and Zubko, S. P., J. Appl. Phys. (1997) 82, 4475. 93. Gaillot, D. P., et al., New J. Phys. (2008) 10, 115039. 94. Khoo, I. C., et al., Opt. Lett. (2006) 31, 2592. 95. Gordon, J. A., and Ziolkowski, R. W., Opt. Express (2007) 15, 2622. 96. Huang, X. G., et al., Langmuir (2007) 23, 8695. 97. Li, W., et al., Langmuir (2008) 24, 13772.

DECEMBER 2009 | VOLUME 12 | NUMBER 12

69